Thiophosphate Phase Diagrams Developed in Conjunction with the Synthesis of the New Compounds KLaP2S6, K2La(P2S6)1/2(PS4), K3La(PS4)2, K4La0.67(PS4)2, K9-xLa1+x/3(PS4)4 (x = 0.5), K4Eu(PS4)2, and KEuPS4
Evenson; Peter K. Dorhout; Inorganic Chemistry 40 (2001) 2884–2891; doi:10.1021/ic000596r

data_4319727
_publ_section_title
;
 Thiophosphate Phase Diagrams Developed in Conjunction with the Synthesis
 of the New Compounds KLaP2S6, K2La(P2S6)1/2(PS4), K3La(PS4)2,
 K4La0.67(PS4)2, K9-xLa1+x/3(PS4)4 (x = 0.5), K4Eu(PS4)2, and KEuPS4
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2884
_journal_page_last               2891
_journal_paper_doi               10.1021/ic000596r
_journal_volume                  40
_journal_year                    2001
_chemical_formula_sum            'Eu K P S4'
_chemical_formula_weight         350.27
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           62
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-P 2ac 2n'
_symmetry_space_group_name_H-M   'P n m a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   16.7816(15)
_cell_length_b                   6.6141(6)
_cell_length_c                   6.5142(6)
_cell_measurement_temperature    168(2)
_cell_volume                     723.04(11)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-93 (Sheldrick, 1993)'
_computing_structure_solution    'SHELXS-86 (Sheldrick, 1990)'
_diffrn_ambient_temperature      168(2)
_diffrn_measurement_device       'Bruker CCD'
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0581
_diffrn_reflns_av_sigmaI/netI    0.0475
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       8
_diffrn_reflns_limit_l_min       -8
_diffrn_reflns_number            4521
_diffrn_reflns_theta_max         28.30
_diffrn_reflns_theta_min         2.43
_exptl_absorpt_coefficient_mu    10.504
_exptl_absorpt_correction_type   SADABS
_exptl_crystal_colour            'brown, clear'
_exptl_crystal_density_diffrn    3.218
_exptl_crystal_description       plate
_exptl_crystal_F_000             644
_exptl_crystal_size_max          0.03
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.09
_refine_diff_density_max         1.047
_refine_diff_density_min         -1.209
_refine_diff_density_rms         0.265
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_all   1.069
_refine_ls_goodness_of_fit_obs   1.097
_refine_ls_matrix_type           full
_refine_ls_number_parameters     40
_refine_ls_number_reflns         977
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.069
_refine_ls_restrained_S_obs      1.097
_refine_ls_R_factor_all          0.0552
_refine_ls_R_factor_obs          0.0368
_refine_ls_shift/esd_max         0.000
_refine_ls_shift/esd_mean        0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0308P)^2^+3.2900P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.0749
_refine_ls_wR_factor_obs         0.0687
_reflns_number_observed          787
_reflns_number_total             977
_reflns_observed_criterion       >2sigma(I)
_cod_data_source_file            ic000596r_7.cif
_cod_data_source_block           KEuPS4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Orthorhombic' changed to
'orthorhombic' according to the built-in table from CIF Core
dictionary named 'cif_core.dic' version 2.4.1 from 2010-06-29.

Automatic conversion script
Id: cif_fix_values 1646 2011-03-28 12:23:43Z adriana 

The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'calc
w=1/[\s^2^(Fo^2^)+(0.0308P)^2^+3.2900P] where P=(Fo^2^+2Fc^2^)/3' was
changed to 'calc'. New tag '_refine_ls_weighting_details' was
created. The value of the new tag was set to
'w=1/[\s^2^(Fo^2^)+(0.0308P)^2^+3.2900P] where P=(Fo^2^+2Fc^2^)/3'.

Automatic conversion script
Id: cif_fix_values 3143 2015-03-26 13:38:13Z robertas 
;
_cod_database_code               4319727